Electron Paramagnetic Resonance (EPR) Spectroscopy K.C. Khulbe1, A.F. Ismail2, T. Matsuura1 1
University of Ottawa, Ottawa, ON, Canada; 2Universiti Teknologi Malaysia, Johor Bahru, Johor, Malaysia
Chapter Outline 1. Introduction 47 2. Fundamentals of EPR 2.1 2.2 2.3 2.4 2.5
Principle of Electron Paramagnetic Resonance Electron Spin and Magnetic Moment 51 Hyperfine Coupling 52 Block Diagram of EPR Spectrometer 52 Spin-Labeling Method 53
3. EPR Applications for the Synthetic Polymeric Membranes
3.1 EPR Applications at the University of Ottawa 54 3.2 Applications of EPR to Study Fouling of RO and UF Membranes
4. Other Examples of EPR Applications 4.1 4.2 4.3 4.4
Aging of Proton Exchange Membranes Study of Carbon Nanotubes 61 Metal Organic Frameworks 63 State of Interfacial Water 64
5. Conclusions 65 References 67
1. Introduction Electron paramagnetic resonance (EPR) spectroscopy, also called electron spin resonance, is a technique that is used to study chemical species with unpaired electrons. EPR spectroscopy plays an important role in the understanding of organic and inorganic radicals, transition metal complexes, and some biomolecules. An electron is a negatively charged particle with certain mass; it mainly has two kinds of movements. The first one is spinning around the nucleus, which brings orbital magnetic Membrane Characterization. http://dx.doi.org/10.1016/B978-0-444-63776-5.00003-6 Copyright © 2017 Elsevier B.V. All rights reserved.
48 Chapter 3 moment. The other is spinning around its own axis, which brings spin magnetic moment. Like most spectroscopic techniques, EPR spectrometers measure the absorption of electromagnetic radiation. The EPR spectrum of a free radical is the simplest of all forms of spectroscopy. If an external magnetic field is not present, the two electron spin states (spin up and spin down) are degenerate. The degeneracy of the electron spin states characterized by the quantum number, ms ¼ 1/2 is lifted by the use of a magnetic field. Transitions between the electron spin levels are induced by radiation at the matching frequency. When a magnetic field is induced, atoms with unpaired electrons spin either in the same direction (spin up) or in the opposite direction (spin down) of the applied field. These two possible alignments with different energies are no longer degenerate. The alignments are directly proportional to the applied magnetic field strength. This is called the Zeeman effect. An unpaired electron interacts with its environment, and the details of EPR spectra depend on the nature of those interactions. The readings can provide information on structural and dynamic information, even from the chemical or physical process, without influencing the process itself. The energy associated with the transition is expressed in terms of the applied magnetic field B, the electron spin g-factor g, and the constant mB, which is called the Bohr magneton. The EPR technique has been widely used to study the structure and function of biological membranes. Biological membranes play a vital role in the cell structure and function. Mass and information transport through the membrane are the most important biological functions, whereas the membranes divide the cell into several different compartments. Researches in the past decades have shown that membranes consist of a laterally heterogeneous lipid bilayer with a large number of embedded protein molecules. The bilayer is heterogeneous either in the way of molecular assembly or in the way of the assembly of molecular aggregates. The molecules and the super molecular aggregates thus interact with each other by different interaction forces and exhibit a variety of characteristics in the transport. The elucidation of the structure and function of the biological membrane has been recognized as a formidable task. Despite its complexity, the EPR technique is considered as one of the most important techniques, both experimentally and biologically. Unlike biological membranes, the application of the EPR technique to investigate the synthetic polymeric membranes is very rare and none can be found for ceramic membranes. This is very surprising, considering the fact that the biomimetic membrane such as aquaporin membrane currently occupies the center position in the development of novel separation membranes. It is attempted in this article to review the EPR applications for the study of synthetic polymeric membranes. The fundamentals of the EPR technique that are outlined before
Electron Paramagnetic Resonance (EPR) Spectroscopy 49 some examples of EPR applications in the synthetic polymeric membranes are shown. Then, the EPR works that have potential in the future investigation of separation membranes are collected from the literature and the problems that should be addressed for the wider applications of the EPR technique are shown.
2. Fundamentals of EPR 2.1 Principle of Electron Paramagnetic Resonance Magnetic moment of the molecule is primarily contributed by unpaired electron (Fig. 3.1). By increasing the external magnetic field, the gap between two energy states is widened until it matches the energy of the microwaves, as represented by the double arrow in the diagram above. At this point the unpaired electrons can move between their two spin states. Since there are typically more electrons in the lower state, due to the MaxwelleBoltzmann distribution, there is a net absorption of energy, and it is this absorption that is monitored and converted into a spectrum (see Fig. 3.2). The upper spectrum below is the simulated absorption for a system of free electrons in a varying magnetic field. The lower spectrum is the first derivative of the absorption spectrum. The latter is the most common way to record and publish EPR spectra. If we are dealing with systems with a single spin like this example, then EPR would always consist of just one line and would have little value as an investigative tool, but several factors influence the effective value of g in different settings. Since the source of an EPR spectrum is a change in an electron’s spin state, it might be thought that all EPR spectra for a single electron spin would consist of one line. However, the interaction of an unpaired electron, by way of its magnetic moment with nearby nuclear spins, results in additional allowed energy states and, in turn, multilined spectra. In such cases, the spacing between the EPR spectral lines indicates the degree of interaction between the
Figure 3.1 Energy levels for an electron spin (ms ¼ 1/2) in an applied magnetic field B0 .
50 Chapter 3
Figure 3.2 Absorption of energy .
unpaired electron and the perturbing nuclei. The hyperfine coupling constant of a nucleus is directly related to the spectral line spacing and, in the simplest cases, is essentially the spacing. Fundamentally EPR is similar to the more widely familiar method of nuclear magnetic resonance (NMR) spectroscopy, with several important distinctions. Although both spectroscopies deal with the interaction of electromagnetic radiation with magnetic moments of particles, there are many differences between the two spectroscopies: 1. EPR focuses on the interactions between an external magnetic field and the unpaired electrons of whatever system it is localized to, as opposed to the nuclei of individual atoms. 2. The electromagnetic radiation used in NMR typically is confined to the radio frequency range between 300 and 1000 MHz, whereas EPR is typically performed using microwaves in the 3e400 GHz range. 3. In EPR, the frequency is typically held constant, whereas the magnetic field strength is varied. This is the reverse of how NMR experiments are typically performed, where the magnetic field is held constant while the radio frequency is varied. 4. Due to the short relaxation times of electron spins in comparison to nuclei, EPR experiments must often be performed at very low temperatures, often below 10K, and sometimes as low as 2K. This typically requires the use of liquid helium as a coolant. 5. EPR spectroscopy is inherently roughly 1000 times more sensitive than NMR spectroscopy due to the higher frequency of electromagnetic radiation used in EPR in comparison to NMR.
Electron Paramagnetic Resonance (EPR) Spectroscopy 51 EPR permits observation of any substance having unpaired electrons. Some examples of substances that exhibit this quality are as follows: 1. Atoms or ions having partially filled inner electron shells that are all of the transition elements of the iron series, rare earth’s and platinum series. 2. Molecules having an odd number of electrons in their outer shells (e.g., NO or ClO2). 3. Molecules with an even number of electrons in their outer shells but with a resultant magnetic moment (e.g., O2). 4. Free radicals, which are naturally or artificially produced. 5. Conduction electrons in metals and acceptors and donors in semiconductors. 6. Modified crystal structure and defects in crystals, e.g., color centers. EPR study is affected by the degree of detail desired and by the type of problem investigated. It is sensitive to the local environment.
2.2 Electron Spin and Magnetic Moment As discussed earlier, an electron is a negatively charged particle with certain mass and has mainly two kinds of movements. The first one is spinning around the nucleus, which brings orbital magnetic moment, and the other is spinning around own axis, which brings spin magnetic moment. Magnetic field of the molecule is primarily contributed by unpaired electron’s spin magnetic moment, which is given by, MS ¼
pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ h SðS þ 1Þ 2p
MS is the total spin angular momentum, S is the spin quantum number, and h is Planck’s constant. In the z direction, the component of the total spin angular moment can only assume two values: h (3.2) 2p the term ms has (2S þ 1) different values: þS, (S 1), (S 2),. S. For single unpaired electron, only two possible values for ms are þ1/2 and 1/2. MSZ ¼ mS $
The magnetic moment, me is directly proportional to the spin angular momentum and one may therefore write me ¼ ge mB MS
The appearance of negative sign is because the magnetic moment of electron is collinear but antiparallel to the spin itself. The term (gemB) is the magnetogyric ratio. The factor ge is known as the free electron g-factor with a value of 2.002 319 304 386 (one of the most
52 Chapter 3 accurately known physical constants). The Bohr magneton, mB, is the magnetic moment for one unit of quantum mechanical angular momentum: mB ¼ ðehÞ=ð4pm Þ e
where e is the electron charge, me is the electron mass. This magnetic moment interacts with the applied magnetic field. The interaction between the magnetic moment (me) and the field (B) is described by E ¼ me B
For single unpaired electron, there will be two possible energy states, this effect is called Zeeman splitting. 1 Eþ1 ¼ gmB B 2 2 1 E1 ¼ gmB B 2 2
In the absence of external magnetic field, Eþ1/2 ¼ E1/2 ¼ 0. In the presence of external magnetic field, as illustrated in Fig. 3.1, with the absorption of radiation, the difference between the two energy states can be written as DE ¼ hv ¼ gmB B
With the intensity of the applied magnetic field increasing, the energy difference between the energy levels widens until it matches with the microwave radiation and results in absorption of photons.
2.3 Hyperfine Coupling Since the source of an EPR spectrum is a change in an electron’s spin state, it might be thought that all EPR spectra for a single electron spin would consist of one line. However, the interaction of an unpaired electron, by way of its magnetic moment, with nearby nuclear spins, results in additional allowed energy states and, in turn, multilined spectra. In such cases, the spacing between the EPR spectral lines indicates the degree of interaction between the unpaired electron and the perturbing nuclei. The hyperfine coupling constant of a nucleus is directly related to the spectral line spacing and, in the simplest cases, is essentially the spacing itself.
2.4 Block Diagram of EPR Spectrometer Fig. 3.3 shows a block diagram for a typical EPR spectrometer. The radiation source usually used is called a klystron. Klystrons are vacuum tubes known to be stable
Electron Paramagnetic Resonance (EPR) Spectroscopy 53
Figure 3.3 Block diagram for a typical electron paramagnetic resonance spectrometer .
high-power microwave sources, which have low-noise characteristics and thus give high sensitivity. A majority of EPR spectrometers operate at approximately 9.5 GHz, which corresponds to about 32 mm. The radiation may be incident on the sample continuously [i.e., continuous wave (cw)] or pulsed. The sample is placed in a resonant cavity, which admits microwaves through an iris. The cavity is located in the middle of an electromagnet and helps to amplify the weak signals from the sample. Numerous types of solid-state diodes are sensitive to microwave energy and absorption lines then can be detected when the separation of the energy levels is equal or very close to the frequency of the incident microwave photons. In practice, most of the external components, such as the source and detector, are contained within a microwave bridge control. Additionally, other components, such as an attenuator, field modulator, and amplifier, are also included to enhance the performance of the instrument.
2.5 Spin-Labeling Method Most chemical and biological samples of interest for EPR spectroscopy lack an inherent stable unpaired electron, the majority of EPR methods rely on the usage of spin-labeling reagents. The radical so introduced is often called a spin label or a spin probe. It is invariably a nitroxide radical, which exhibits a three-line hyperfine structure whose peak shape, splitting, etc., depend on the radical’s environments. The nitroxide label is a monitor of motion. The shape of the EPR signal depends also on the orientation of the magnetic field relative to the axis of the radical. Thus, the spin label method is useful to study the environment of radical, which is the structure of the polymer at a molecular level.
54 Chapter 3
Figure 3.4 Electron paramagnetic resonance spectra of 2,2,6,6-tetramethyl-1-piperidinyloxy solution in water (0.02 wt%) .
Commonly, nitroxides such as derivatives of TEMPO (2,2,6,6-tetramethyl-1piperidinyloxy) are used as they offer high stability of the unpaired electron and exceptional EPR sensitivity combined with facile and versatile moieties for binding to the sample through chemical reactions itself. Fig. 3.4 shows the EPR spectra of TEMPO solution in water (0.02 wt%). The spectra consist of three symmetric peaks since the NO* radical of TEMPO (or with 5-, 12-, and 16-doxylstearic acid derivatives) is freely mobile in the solution. The spectra are isotropic (symmetric) and the value of Hamiltonian parameter, the factor ge is known as the free electron g-factor with a value of 2.002 319 304 386 (one of the most accurately known physical constants) and ǀAǀ (distance between two peaks) is 17 G. All three peaks are almost equal in height and symmetric. Interactions of an unpaired electron with its environment influence the shape of an EPR spectral line. The shape of curves and other properties of the EPR spectra gives the clue for analysis.
3. EPR Applications for the Synthetic Polymeric Membranes 3.1 EPR Applications at the University of Ottawa Khulbe and Matsuura  wrote a review in which they discussed the characterization of synthetic membranes by EPR.
Electron Paramagnetic Resonance (EPR) Spectroscopy 55 The radicals were detected in the polymeric material from which membranes are fabricated and the number of radicals depended on the conditions in which the membranes were fabricated and the environment to which the membranes were exposed. Polymers themselves contain paramagnetic free radicals. It is possible that these radicals may take part in the transportation of gases through the membrane. It is observed that these radicals are affected reversibly with gases (CO2 and CH4). Khulbe et al.  reported that polyphenylene oxide (PPO) radicals are present in PPO powder, and the membranes prepared from PPO contain free radicals that are affected by the conditions of the environment. It was reported that the number of spins/g in membranes is higher than in the PPO powder and it also depends on the characteristics of solvents used for membrane preparation. Generally, the number of spins/g in vacuum is less than in the air. However, no definite conclusion could be drawn due to small quantity of spins (1014 spins/g). It was noticed that in the presence of N2 the number of spins/g (concentration) was more than that in the presence of O2. On the contrary, the number of spins/g was higher in the presence of CH4 than CO2. The permeation rates through the membrane of CO2 and O2 are usually higher than CH4 and N2, respectively. This type of behavior also was observed with sulfonated and brominated PPO membranes . Incorporation of the spin label TEMPO was also attempted by Khulbe et al. . Dense homogeneous PPO membranes were prepared by casting a solution, which consisted of PPO, TEMPO (spin probe), and 1,1,2-trichloroethylene solvent. The solvent was evaporated at 22, 4, and 10 C. Membranes were subjected to EPR spectroscopic study as well as to the permeability measurement of various gases, including O2, N2, CO2, and CH4. It was observed that the intensity of the spin probe decreased with the decrease of temperature used for the preparation of the membrane. The intensity of the spin probe was almost at zero level for the membrane prepared at 10 C in comparison with the EPR signal intensity of the other two membranes prepared at higher temperatures. It could be due to high crystallinity state in the membrane prepared at 10 C or some level of molecular ordering. Authors concluded that 1. The intensity of the spin probe in the PPO membrane depends on the temperature of solvent evaporation during dense membrane preparation. 2. The morphology of the surface on the membrane depends on the temperature used for the preparation of the membrane. 3. Generally, the permeation rate of gases (especially with CO2 and CH4) increases with the decrease in the temperature used for the preparation of membrane. It could be possible that Langmuir sites are most favorable for the CH4 and N2 permeation in PPO membrane. It could be possible that Henry sites are good for selectivity. Gumi et al.  studied activated composite membranes by EPR and reported that EPR is a useful tool for the characterization of activated composite membranes.
56 Chapter 3 Another example of the incorporation of spin label is the work by Khulbe et al.  who prepared dense membranes from poly(phenylene oxide) (PPO) by blending spin probes (TEMPO, 5-, 12-, and 16-doxylstearic acid) in the casting solution. It was noticed that the shape and size of the probe influence the EPR spectra of the NO* radical in the PPO membrane. Unexpectedly, from the shape of the EPR signal it was noticed that the NO* radical of TEMPO in PPO membrane was more mobile than in water media. However, the motion of the NO* radical of 16-doxylstearic acid was higher than that of NO* radical of 5- and 12-doxylstearic acid when the radicals were in the PPO membrane. This could be due to the inductive effect from COOH group. The Hamiltonian parameters of the EPR signal indicated that all the probes were not randomly distributed in the PPO membrane, but some probes were distributed in the polymer in orderly fashion. Khulbe et al.  studied the structure of the skin layer of asymmetric cellulose acetate (CA) RO membranes with TEMPO probe. It was observed that the mobility of TEMPO in the asymmetric membrane shrunk at 90 C was the same as TEMPO in a dense homogeneous membrane prepared from the same casting solution. Authors reported the following conclusions 1. The pore sizes of the asymmetric membranes are larger when they were shrunk at lower temperatures 2. The space in the polymer network (the origin of the network pore) in the dense film was smaller when no swelling agent is added to the casting solution 3. The space in the polymer network in the dense film was smaller when the membrane was dry In another study, Khulbe et al.  used EPRspectroscopy as a method to study membrane fouling during ultrafiltration (UF). Bovine serum albumin (BSA) and polyethylene oxide, with and without TEMPO (spin probe), solutions in water were used as the feed in the UF experiments. Asymmetric membranes were prepared by phase inversion technique using casting solutions of polyethersulfone (PES) in n-methyl pyrrolidone. Polyvinyl pyrrolidone was added as a nonsolvent additive. The following conclusions were reported. 1. Deposition of BSA on the surface and inside the pore during UF is in a specific orientation (manner). However, the orientation of BSA molecule on the surface is different from that of the BSA molecule inside the pore. 2. The packing density of BSA molecules inside the pore depends on the particular pore size and feed pressure. At higher feed pressure, the denser packing moves toward smaller pore size. 3. Fouling depends on the structure of solute. EPR spectroscopy technique was also used to study CA membranes for reverse osmosis (RO) and PES membranes for UF . TEMPO was used as a spin probe that was
Electron Paramagnetic Resonance (EPR) Spectroscopy 57 brought into the membranes by immersing the membranes into solutions involving TEMPO, or by blending TEMPO into membrane casting solutions. The following conclusions were reported: 1. EPR technique can be used to study the structure and the transport of RO and UF membranes. 2. Water may flow through the pores of PES membranes. The sizes of pores are those of UF membranes. Unlike CA, the polymer matrix of PES membrane is a little swollen or not at all swollen by water and continuous channels through which water flows cannot be formed. In CA, spaces in water swollen polymer matrix were the primary provider of continuous flow channels that contribute to the separation of salt and small organic molecules. In the absence of such water channels, PES membranes cannot act as RO membranes. Khulbe et al.  reported the EPR study on the structure and transport of asymmetric aromatic polyamide membranes. TEMPO was used as a spin probe that was brought into the membrane by (a) immersion of the membranes in aqueous TEMPO solutions, (b) RO experiments with feed solutions involving TEMPO, or (c) blending TEMPO in casting solutions. The membranes were tested for the separation of sodium chloride and TEMPO from water by RO. It was concluded that aromatic polyamide membranes contain water channels in the polymer matrix like CA membranes. A comparison was made with other RO membranes (CA) and UF membranes (PES). It was suggested that the EPR technique can be used to study the structure of UF and RO membranes. The presence of water channels in the polymer matrix seems indispensable for the RO membrane.
3.2 Applications of EPR to Study Fouling of RO and UF Membranes Membrane fouling and aging were studied by the other groups using EPR technique. Oppenheim et al.  spin-labeled hen egg lysozyme (HEL) with 3-maleimido-proxy at two positions of macromolecule. HEL solution was ultrafiltered in a cross-flow UF apparatus for 2 h using polysulfone UF membrane of molecular weight cutoff (MWCO) ¼ 10 kDa. Then, spin-labeled HEL in saline buffer solution and on the UF membrane were subjected to EPR analysis. Figs. 3.5 and 3.6 show the EPR signals obtained from HEL in the buffer solution and HEL in the UF membrane, respectively. The peaks indicated in Fig. 3.6 by arrows were ascribed by the authors to the spinespin interaction between two spin labels of HELs confined in narrow pore channels. When HEL was ultrafiltered by UF membrane of MWCO ¼ 30 kDa, the EPR signal was similar to that of HEL in the buffer solution, indicating the pores of the latter membrane (MWCO ¼ 30 kDa) were not blocked by HELs. RO and UF membranes are often cleaned chemically by contacting the membranes with hypochlorite solution. It has long been suggested that degradation of polymer takes place
58 Chapter 3
Figure 3.5 Electron paramagnetic resonance signal from the hen egg lysozyme in buffer solution .
during the membrane cleaning due to radical formation . To confirm this hypothesis Oliveira et al. studied, using EPR technique, the aging of polyamide thin film composite membrane during the chemical cleaning by hypochlorite solution changing the hypochlorite concentration as well as pH .
Figure 3.6 Electron paramagnetic resonance signal from the hen egg lysozyme in the UF membrane (MWCO 10 kDa) pore .
Electron Paramagnetic Resonance (EPR) Spectroscopy 59
Figure 3.7 Electron paramagnetic resonance spectra taken after the membrane was immersed in bleach solution of (a) 80, (b) 50, and (c) 20 v/v% .
Dow Filmtech NF 270 membrane was immersed in bleach solution (NaClO3) before the membrane was dried and transferred into a quartz tube for EPR observation. The intensity of the EPR signal has increased with an increase of bleach concentration as shown in Fig. 3.7, whereas the radical formation was suppressed by increasing pH (Fig. 3.8). Unfortunately, the radical species could not be identified due to the absence of the hyperfine structure. They have also studied the effect of the membrane exposure to the sunlight on the radical formation and the radical formation during the ultraviolet (UV) membrane surface grafting and confirmed that the membrane degradation occurred under an excessive UV irradiation.
4. Other Examples of EPR Applications 4.1 Aging of Proton Exchange Membranes The degradation of proton exchange membranes (PEMs) is an important subject in the fuel cell application. As a typical PEM Nafion was chosen and its degradation mechanism was studied by EPR when Nafion was neutralized by Cu(II), Fe(II), and Fe(III) ions . When Nafion was neutralized by FeSO4 and irradiated by UV, the signal from ROCF2CF2$ radical was detected and its intensity increased with the UV irradiation time (Fig. 3.9). Remarkably, the signal was also observed even before the UV irradiation, indicating radical formation in the presence of Fe(II) without UV irradiation. At the same time the formation of Fe(III) was detected.
60 Chapter 3
Figure 3.8 Electron paramagnetic resonance spectra after the membrane was immersed in 50 v/v % bleach solution at (a) pH ¼ 8 and (b) pH ¼ 9 .
Figure 3.9 Electron paramagnetic resonance signal for ROCF2CF2$ radical when neutralized by Fe(II) .
Electron Paramagnetic Resonance (EPR) Spectroscopy 61 Thus, the radical formation and polymer degradation are possible in the presence of metal ions such and Cu(II), Fe(II), and Fe(III) even without UV irradiation.
4.2 Study of Carbon Nanotubes Much attention has been paid to carbon nanotubes (CNTs) to apply them for separation membranes due to their extraordinarily high permeability for water and gas. Many attempts have also been made to incorporate them in the mixed matrix membranes (MMMs) . The study of CNTs by EPR was conducted even before the announcement of the unusual permeation characteristics of CNTs by Hinds et al. . Multiwalled CNTs were embedded in styrene-polyisoprene-polystyrene (SIS) block copolymer and its EPR spectra were recorded . The resonance spectrum of SIS-CNTs composite is featured by a strong and symmetric peak at g ¼ 2.06 and the resonance line width of 102 G, which was ascribed to the strongly interacting localized and itinerant electrons, in the so-called bottleneck state. The double integral of the resonance line called S is proportional to the susceptibility. When S is plotted versus temperature (Fig. 3.10), S depends only weakly on temperature when the CNT content in the composite is low, but S depends strongly on temperature when the CNT content is high. Since susceptibility S of localized electron is temperature dependent, whereas S of delocalized electron is temperature independent, Fig. 3.10 means that the amount of localized electron is very small when the CNT content is low. These localized electrons were most likely those of Feþ3 ions in the residual catalyst of CNT synthesis. As the CNT loading increases, the amount of
Figure 3.10 Temperature dependence of S .
62 Chapter 3 localized electrons (paramagnetic defects) increases and so does the temperature dependency. This means these paramagnetic defects are localized either within CNTs themselves or at the CNTsepolymer interface. Another study on CNTs was done by Rao et al. . Double walled carbon nanotubes of 0.45 nm average diameter were embedded in VP 15 molecular sieve (zeolite) nanochannels and subjected to EPR at temperatures 4.2, 20, 40, 60, and 75K. From Fig. 3.11, for all temperatures a symmetric EPR signal is observed at gc z 2.0028 with a corresponding density z1019 g1. Generally, for single walled carbon nanotubes (SWCNTs) and MWCNTs of much larger diameter (more than 1 nm) different types of EPR signals are observed, i.e., (1) signal centered at gc ¼ 2.0 coming from the residual metal catalytic particles, (2) gc ¼ 2.07 coming from the conduction electron spin resonance, and (3) gc ¼ 2.00 coming from localized electron spins. Therefore, Fig. 3.11 excludes the possibility of the presence of conduction electrons. The electrons are localized in the defect on the CNTs.
Figure 3.11 Electron paramagnetic resonance signal of carbon nanotubes embedded in zeolite at different temperatures .
Electron Paramagnetic Resonance (EPR) Spectroscopy 63
4.3 Metal Organic Frameworks Much attention is also paid to metal organic frameworks (MOFs) due to its unique structures that allow strong adsorption of gaseous molecules . They are also embedded in polymeric membrane to form MMMs for gas and liquid separation . MOF expands in their crystalline structure when guest molecules are adsorbed in it, whereas it shrinks when the molecules are desorbed, a phenomena known as “breathing.” It was confirmed by EPR that similar structural change takes place when temperature changes from high (HT) to low (LT) and vice versa. Cr(III)-doped aluminum-based MIL-53 was synthesized where the main metal ion is Al (99%), whereas the rest of 1% is Cr. The sample was further calcinated and evacuated to remove water and residual organic acid and it was called MIL-53(Al/Cr)deh, where deh means dehydration. The Q-band EPR spectra of MIL-53(Al/Cr)deh taken at different temperatures are shown in Fig. 3.12. At 295K (Fig. 3.12(a,b)), three singularities (q ¼ 0 degree, 42 degree, and 90 degree) of the central MS ¼ 1/2 4 ½ transition appear between 1170 and 1320 mT. Furthermore, two single q ¼ 90 degree edge singularities of the MS ¼ 3/2 4 ½ transitions are observed at 940 and 1540 mT without splitting, indicating an axially symmetric tensor (E z 0). Then, the ratio of spin Hamiltonian parameters E/D becomes nearly equal to
Figure 3.12 Electron paramagnetic resonance spectra of MIL-53(Al/Cr)deh at (a) experimental, (b) simulated at 295K, (c) experimental, and (d) simulated at 5K .
64 Chapter 3 zero, hence these signals are assigned to CrO4(OH)2 octahedral (Fig. 3.13(a)) in the HT phase of MIL-53(Al/Cr)deh. On the other hand, at a lower temperature of 5K, the Q-band spectrum transformed to rhombic nature (Fig. 3.12(c,d)) and the signals at 940 and 1540 mT disappeared, which means the ratio of spin Hamiltonian parameters E/D is no longer zero (by simulation E/D ratio was found to be 0.236), suggesting the lowering in the symmetry of CrO4(OH)2 octahedrons (see Fig. 3.13(b)). It was further proposed that high to low temperature transition occurs at temperatures between 150 and 60K, whereas the transformation from low to high transition occurs at the temperatures between 330 and 375K, indicating the large thermal hysteresis. As well about 20% of the material does not undergo the transition high to low temperature.
4.4 State of Interfacial Water Two polypeptides, 26-residue polypeptide (n3) and 14-mer long proline model peptide (PPm3), were spin labeled and dissolved in vitrified solvent (concentrated aqueous sucrose or glycerol solution) or confined in two mesoporous silica materials, SBA15a
Figure 3.13 Schematic presentation of MIL-53(Al/Cr)deh structure, (a) 295K, (b) 5K .
Electron Paramagnetic Resonance (EPR) Spectroscopy 65 and SBA15b, with pore diameters of 7.6 and 6.1 nm, respectively. Then, they were subjected to several EPR studies including double electron resonance, electron spin echo, and electron spin echo envelope modulation (ESEEM). As well, H2O was sometimes changed to D2O . The parameter p(D2O) measured by ESEEM shows the accessibility of water, especially D2O, within the van der Waals contact distance of c. 0.35 nm from the spin label. As shown in Table 3.1, p parameter does not change in the vitrified solvent or in the pore of SBA 15a and SBA 15b. Only when the peptide PPm3 was in the vitrified solvent containing 40% glycerol, the accessibility was nearly doubled. On the other hand, the parameter Cex, which indicates the density of water (D2O in this case) within the range of 2 nm of the spin label is remarkably different, depending on the confinement in the nanopore. The values for both n3 and PPm3 are in the order of SBA 15b > SBA 15a > vitrified solvent and remarkably high when the polypeptides are confined in SBA 15b with the nanopores of the smaller diameter. Thus, this result confirms that there is density profile in the vicinity of the spin-labeled polypeptide, indicating the presence of special water near polypeptides that represent proteins, so-called “biological surface water.” The importance of such water for sustaining “life” is well recognized. The presence of special water in RO membrane, most likely in the membrane pore, has long been recognized by differential scanning calorimetric (DSC) experiments . Thus, EPR can possibly be a powerful tool to sense the presence of special interfacial water in the membrane pore.
5. Conclusions It was shown that the EPR technique is a powerful tool to study the synthetic polymeric membranes by showing: 1) Radicals are present in the synthetic polymeric membrane. Table 3.1: p Parameter and density (Cex) profile in the vicinity of spin-labeled polypeptide. p 26-residue polypeptide (n3) in SBA 15a n3 in SBA 15b n3 in 40% sucrose solution 14-mer long proline model peptide (PPm3) in SBA 15a PPm3 in SBA 15b PPm3 in 40% glycerol solution
0.156 0.142 0.215
42.3 12.8 28.6
66 Chapter 3
1) 2) 3)
1.1) The concentration of radicals is different depending on the conditions by which membranes are fabricated. The macromolecular radicals in the membrane may lead to the degradation of polymer by radical reactions. 1.2) The radical concentration increases during the chemical cleaning of the membrane, leading to polymer degradation. The radical concentration also increases by exposure to sunlight and during the surface modification by UV grafting. The spin-labeling technique is a powerful tool to characterize the membrane morphology. In particular, 2.1) The order in the macromolecular alignment in the membrane can be detected at the molecular level, which might affect the membrane selectivity in gas separation. 2.2) The difference in the nature of the pores in RO and UF membranes can be identified. Water passes through the swollen intersegmental space (network pores) in the skin layer of the CA RO membrane, whereas in the PES UF membrane water flows through pores formed between the polymer aggregates (aggregate pores). 2.3) The network pores of the CA membranes shrink when the membrane is annealed. 2.4) EPR technique confirms that membrane fouling takes place by protein molecules that are densely packed in the membrane pores. It was shown by some other examples that Radicals were found in the Nafion PEMs when its sulfonic group was partially neutralized by Cu or Fe ions, causing the degradation of the PEMs. It was found that the electron was highly localized in the CNT itself, in the space between CNT and polymer matrix, or in the defect of CNTs. Hysteresis was observed between the expansion of MOF at the HT and shrinkage at the LT, which resembles the breathing of MOF that occurs by adsorption and desorption of guest molecules. The density profile was detected near protein molecules that are confined in nanochannels. This proves the presence of the interfacial water at the protein/water interface.
It should also be noted that the EPR applications for the synthetic polymeric membranes, although they can give some insights into the membrane structure and performance, all of the currently available works lack precise analysis of the hyperfine structures of the EPR signals. On the other hand, in the other works, the hyperfine structures of EPR signals were analyzed more rigorously, giving details of the EPR signal sources. Unfortunately, however, it is very difficult to understand how the EPR parameters can be interpreted due to the complexity of the EPR theory.
Electron Paramagnetic Resonance (EPR) Spectroscopy 67 As well, EPR technique has the following drawbacks compared to the other characterization techniques. 1) It is impossible to obtain two-dimensional (2D) or three-dimensional (3D) images of the membrane surface (and the cross-section) unlike scanning electron microscope, transmission electron microscope, and atomic force microscope. 2) Currently, it is impossible to investigate the surface of the membrane separately from the bulk, unlike FTIR-ATR, XPS, EDX, and contact angle measurement. 3) Hence, the data are affected by the bulk structures under the top surface layer that governs the performance of the asymmetric membrane, similar to XRD, DSC, TGA, and measurement of mechanical strength. Thus, the complication involved in the theoretical interpretation of EPR, absence of 2D and 3D images taken by the EPR technique and difficulty in the surface observation is now hampering the wider usage of the EPR technique to investigate the synthetic polymeric membrane despite its enormous potential to reveal the details of the membrane structure.
References  UC Davis ChemWiki, http://chemwiki.ucdavis.edu/Physical_Chemistry/Spectroscopy/Magnetic_ Resonance_Spectroscopies/Electron_Paramagnetic_Resonance/EPR%3A_Theory.  What is EPR spectroscopy?: University of Texas at Austin. http://epr.cm.utexas.edu/WhatIsEPR.html.  Khulbe KC, Hamad F, Feng C, Matsuura T, Gumi T, Palet C. ESR spectra of spin probe in PPO membrane. Polymer 2003;44:695e701.  Khulbe KC, Matsuura T. Characterization of synthetic membranes by Raman spectroscopy, electron spin resonance, and atomic force microscopy; a review. Polymer 2000;41:1917e35.  Khulbe KC, Chowdhury G, Matsuura T, Lamarche G. Characterization of PPO [poly(phenylene oxide) ] powder and membranes from it by ESR technique. J Membr Sci 1997;123:9e15.  Khulbe KC, Chowdhury G, Kruczek B, Vujosevic R, Matsuura T, Lamarche G. Characterization of the PPO dense membrane prepared at different temperatures by ESR, atomic force microscope and gas permeation. J Membr Sci 1997;126:115e22.  Gumi T, Valiente M, Khulbe KC, Palet C, Matsuura T. Characterization of activated composite membranes by solute transport, contact angle measurement, AFM and ESR. J Membr Sci 2003;212:123e34.  Khulbe KC, Matsuura T, Lamarche G, Lamarche A-M, Choi C, Noh SH. Study of the structure of asymmetric cellulose acetate membranes for reverse osmosis using electron spin resonance (ESR) method. Polymer 2001;42:6479e84.  Khulbe KC, Matsuura T, Singh S, Lamarche G, Noh SH. Study on fouling of ultrafiltration membrane by electron spin resonance. J Membr Sci 2000;167:263e73.  Khulbe KC, Matsuura T, Feng SCY. Study on cellulose acetate membranes for reverse osmosis and polyethersulfone membranes for ultrafiltration by electron spin resonance technique. Desalination 2002;148:329e32.  Khulbe KC, Feng C, Matsuura T, Lamarche G, Lamarche A-M. Study of the structure of asymmetric polyamide membranes for reverse osmosis using the electron spin resonance (ESR) method. Desalination 2003;154:1e8.
68 Chapter 3  Oppenheim SF, Buettner GR, Dordick JS, Rodgers VGJ. Applying electron paramagnetic resonance spectroscopy to the study of fouling in protein ultrafiltration. J Membr Sci 1994;96:289e97.  Kwon Y-N, Leckie JO. Hypochlorite degradation of crosslinked polyamide membranes I. Changes in chemical/morphological properties. J Membr Sci 2006;283:21e6.  Oliveira FRP, Matos CT, Moura JJG, Portugal CAM, Crespo JG. Study of membrane ageing and grafting mechanisms using electron paramagnetic resonance. Desalination Water Treat 2011;27:150e8.  Kadirov MK, Bosnjakovic A, Schlick S. Membrane-derived fluorinated radicals detected by electron spin resonance in UV-irradiated nafion and Dow ionomers: efffect of counterions and H2O2. J Phys Chem B 2005;109:7664e70.  Yang HY, Han ZJ, Yu SF, Pey KL, Osrikov K, Karnik R. Carbon nanotube membranes with ultrahigh specific adsorption capacity for water desalination and purification. Nat Commun 2013;4. http://dx.doi.org/ 10.1038/ncomms3220. Article number: 2220.  Hinds BJ, Chopra N, Rantell T, Andrews R, Gavalas V, Bachas LG. Aligned multiwalled carbon nanotube membranes. Science 2004;303:62e5.  Chipara M, Zaleski JM, Hui D, Du C, Pan N. Electron spin resonance on carbon nanotubes-polymer composites. J Polym Sci Part B 2005;43:3406e12.  Rao SS, Stesmans A, Noyen JV, Jacobs P, Sels B. Electron spin resonance investigation of ultra-small double walled carbon nanotubes embedded in zeolite nanochannels. J Phys Condens Matter 2011;23:455801. 6 pp.  Hartmann M, Kunz S, Himsl D, Tangermann O. Adsorptive separation of isobutene and isobutane on Cu3(BTC)2. Langmuir 2008;24:8634e42.  Mendt M, Jee B, Stock N, Ahnfeldt T, Hartmann M, Himsl D, Po¨ppl A. Structural phase transitions and thermal hysteresis in the metalorganic framework compound MIL-53 as studied by electron spin resonance spectroscopy. J Phys Chem C 2010;114:19443e51.  Lai Y-C, Chen Y-F, Chiang Y-W. ESR study of interfacial hydration layers of polypeptides in water-filled nanochannels and in vitrified bulk solvents. PLoS One 2013;8:e68264. p. 130.  Taniguchi Y, Horigome S. The states of water in cellulose acetate membranes. J Appl Polym Sci 1975;19:2743e8.